Author’s Accepted Manuscript Electrochemical biosensing platform based on Amino acid Ionic liquid functionalized graphene for ultrasensitive biosensing applications Xianbo Lu, Xue Wang, Jing Jin, Qing Zhang, Jiping Chen www.elsevier.com/locate/bios
PII: DOI: Reference:
S0956-5663(14)00449-7 http://dx.doi.org/10.1016/j.bios.2014.06.036 BIOS6870
To appear in: Biosensors and Bioelectronic Received date: 8 April 2014 Revised date: 5 June 2014 Accepted date: 10 June 2014 Cite this article as: Xianbo Lu, Xue Wang, Jing Jin, Qing Zhang and Jiping Chen, Electrochemical biosensing platform based on Amino acid Ionic liquid functionalized graphene for ultrasensitive biosensing applications, Biosensors and Bioelectronic, http://dx.doi.org/10.1016/j.bios.2014.06.036 This is a PDF file of an unedited manuscript that has been accepted for publication. As a service to our customers we are providing this early version of the manuscript. The manuscript will undergo copyediting, typesetting, and review of the resulting galley proof before it is published in its final citable form. Please note that during the production process errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain.
Electrochemical biosensing platform based on amino acid ionic liquid
functionalized graphene for ultrasensitive biosensing applications
Xianbo Lu*, Xue Wang, Jing Jin, Qing Zhang, Jiping Chen
Dalian Institute of Chemical Physics, Chinese Academy of Sciences, Dalian, 116023, China.
In this study, a facile non-covalent method was developed for preparing water-soluble graphene
with excellent electronic conductivity. Room temperature ionic liquids (ILs) with high ionic
conductivity were used for the non-covalent surface functionalization of graphene through ππ
stacking interactions. Compared to other ILs used, amino acid ionic liquids (AAILs) were found
to be the most effective for improving the dispersion of graphene in water phase.
Electrochemical and spectroscopic results confirmed that the obtained AAIL functionalized GR
can retain the excellent electronic conductivity of pristine graphene without damaging the
graphene lattice. The obtained water-soluble graphene (GR-AAIL) was exemplified to fabricate
an electrochemical biosensor using tyrosinase as a model enzyme, and the sensitivity (12600 mA
cm-2 M-1) of GR-AAIL based biosensor was about 17 times higher than that of graphene oxide
and other nanomaterial based biosensor, displaying its unprecedented high sensitivity for
E-mail: [email protected]
, [email protected]
biosensing. The detection limit for catechol (one important environmental pollutants) reached as
low as 8 nM with a response time of 3 s and a linear range from 25 nM to 11100 nM. The AAIL-
GR based biosensor also demonstrated good reproducibility, repeatability, selectivity, long-term
stability and high recovery for catechol detection. Amino acid ionic liquid functionalized
graphene proves to be a robust and versatile electrochemical biosensing platform for fabricating
biosensors with excellent performance.
KEYWORDS: Biosensor, Graphene, Amino Acid Ionic liquids, Electronic conductivity,
Graphene (GR), the archetypal 2D nanomaterial, is a single atomic layer of carbon with
extraordinary properties including exceptionally high electronic carrier mobilities, thermal
conductivity, and mechanical strength. GR is expected to find potential applications in many
fields such as electronics, sensors, biosensors, optoelectronics, batteries, supercapacitors,
catalysis, chemical and biological sensing (Ponomarenko et al., 2008; Wu et al., 2012a; Liu et al.,
2013a; Liu et al., 2013b; Gholivandn and Khodadadian, 2014). As shown with carbon nanotubes,
the dispersion of nanomaterials in solution is crucial to advancing many applications (Baughman
et al., 2002; Sun et al., 2002). Owing to their hydrophobic nature, the direct dispersion of GR
sheets in water has been generally considered unattainable. GR sheets, which have a high
specific surface area, tend to form agglomerates or even restack to form graphite through van der
Waals interactions, making further processing difficult. The functionalization of GR has been
considered to be important for improving their solubility, self-assembly properties, and
applications in devices. The commonly used method for dispersing GR sheets is to utilize the
hydrophilic groups on GR surface. Usually water-soluble graphene oxide (GO) or functionalized
graphene (e.g. carboxylic or hydroxy graphene) is used (Park and Ruoff, 2009; Zhou et al., 2013),
however, it is electrically insulating or has poor electronic conductivity. To restore the electronic
conductivity, GO requires complicated chemical reduction or annihilation under high
functionalization of graphene (Si and Samulski, 2008) suffers from the same problem as GO (i.e.
the decreased electronic contuctivity) as all these techniques use the hydroxyl or carboxylic
groups on graphene surface. And these structural defects on GR surface inevitably alter the
electronic conductivity of graphene. A viable alternative to form GR dispersion is the non-
covalent functionalization of GR (Xu et al., 2008; Malig et al., 2012). GR might be stabilized by
some amphiphilic polymers or surfactants (Lotya et al., 2009) to form a stable dispersion without
destroying the intrinsic structure of GR. However, one potential risk of the above method is that
the electronic conductivity of GR may be affected by the poor conductivity of remained
polymers or surfactants. Using amphiphilic room temperature ionic liquids (RTILs) may be
preferred for the dispersion and functionalization of GR as ionic liquids possess excellent ionic
Room temperature ionic liquids are compounds consisting entirely of ions that exist in the liquid
state around room temperature (Lu et al., 2006; Moulthrop et al., 2005). As novel attractive green
solvents, they possess unique properties such as negligible vapor pressure, wide potential
windows, high thermal and chemical stability, and excellent ionic conductivity. The physical
properties of RTILs, such as the oil/water partition coefficient, can be adjusted by incorporating
(Malig et al., 2012) to afford reduced graphene oxide (r-GO). Covalent
different organic cations and inorganic or organic anions. Some biocompatible ionic liquids, such
as 1-butyl-3-methyl-imidazolium tetrafluoroborate, have been used for biosensors (Lu et al.,
2006) or biocatalysis (Lou et al., 2004) with increased enzymatic activity and stability.
In this communication, we prepared stable aqueous dispersions of GR sheets without sacrificing
its electronic conductivity and structure integrity by using amphiphilic anino acid ionic liquids
(AAILs) as a stabilizer, since the imidazole moiety has been reported to have strong affinity with
the basal plane of graphite viaπ-stacking. Up to date, noncovalent functionalization of GR sheets
using AAILs throughπ-π interactions has not been addressed in the literature. Of significant is
that, unlike conventional polymers or surfactants, these amphiphilic ionic liquids possess high
ionic conductivity. Once these ionic liquids are purposely retained, they are expected to provide
better conductivity compared to conventional polymer or surfactants stabilizer. On the other
hand, these ionic liquids can be easily gotten rid of by filtration and washing if they are not
needed anymore. Based on the obtained AAIL-functionalized graphene (AAIL-GR), an
electrochemical tyrosinase biosensor was fabricated (tyrosinase as a model enzyme), and the
unprecedented high sensitivity for biosensing was displayed. The AAIL-GR based biosensor also
demonstrated good reproducibility, selectivity, long-term stability and low detection limit for
catechol detection. The fabricated biosensor for real water sample detection was also
investigated with high recovery. Amino acid ionic liquid functionalized graphene proves to be a
robust electrochemical biosensing platform for fabricating biosensors with excellent performance.
2. Materials and Methods
GR (purity~99％) and GO (purity~99％) were from Nanjing XFNANO Materials Tech Co., Ltd
(China). Chitosan (Chi, minimum 85% deacelytated) and tyrosinase (from mushroom, >1000
units mg-1) were purchased from Sigma (USA). Phenol and other chemicals (analytical grade)
were purchased from Tianjin Kermel Chemical Regent Company (China). Tetrabutyl
phosphonium methanesulfonate, 1-Ethyl-3-methylimidazolium tetrafluoroborate, 1-Butyl-3-
bis(trifluoromethylsulfonyl)amide (purity>98%) were purchased from Sigma-Aldrich. Other IL
(purity>98%) were obtained from Dalian Institute of Chemical Physics, Chinese Academy of
Sciences (China). Table 1 lists these twelve different kinds of ILs selected for investigation.
2.2. Preparation of the GR-IL nanocomposite
Twelve kinds of ILs in table 1 were tesed respectively to improve the dispersion of GR in water
phase. The GR-IL nanocomposite was prepared as follows: An aliquot of GR (usually 0.4 mg)
was mixed with an aqueous solution of ILs (1ml, the concentration of ILs may be adjusted from
0.25 mg ml-1 to 5.0 mg mL-1 for optimization according to the property of ILs and the dispersion
results of GR) with the aid of ultrasonication and vibration for 15 min. The solution containing
0.4 mg ml-1 GR and 3.0 mg ml-1 AAILs was used for the demonstration of images in Figure 1.
The solution containing 0.2 mg ml-1 GR and 0.25 mg ml-1 AAIL was used for FTIR and
electrochemical impedance spectroscopy (EIS) characterization of AAIL-GR.
2.3. TEM and FT-IR
TEM images of GR and GO were obtained with a transmission electron microscope JEM-
2000EX (JEOL, Japan) with an accelerating voltage of 120 kV. FT-IR
spectra of GR, GO,
EMIMAla, and GR-EMIMAla were recorded by using a Spectrum GX apparatus (Perkin--Elmer
2.4. Electrochemical impedance spectroscopy measurements
EIS measurements were performed by using a PGSTAT 302N (Autolab, Switzerland)
workstation in a 1.0 mmol L−1 K3[Fe(CN)6]/K4[Fe(CN)6] (1:1) solution containing 0.5 mol L−1
KNO3 supporting electrolyte, and the results were plotted in the form of complex plane diagrams
(Nyquist plots) with a frequency range from 0.1 Hz to 10 kHz. The electrodes for EIS
measurements were prepared by a similar procedure for the preparation of enzyme electrodes.
The solution compositions for the preparation of different electrodes were as follows: GR-
Chi/GC electrode (0.2 mg ml-1 GR and 0.3 mg ml-1 Chitosan), GO-Chi/GC (0.2 mg ml-1 GO and
0.3 mg ml-1 Chitosan), GR-EMIMAla-Chi/GC (0.2 mg ml-1 GR, 0.25 mg ml-1 EmimAla and 0.3
mg ml-1 Chitosan), and Chi/GC (0.3 mg ml-1 Chitosan).
2.5. Amperometric measurements of biosensors
Amperometric (I-t) measurements were carried out based on three electrode systems by using a
CHI 440B electrochemical workstation (CHI Instruments Inc., USA). The enzyme electrodes for
I-t measurements were prepared as follows. After optimization of the experimental conditions,
the final solution (pH 7.0) containing tyrosinase (2.5 mg mL-1), GR-EMIMAla (0.2 mg mL-1 GR
and 0.25 mg mL-1), and chitosan (1.5 mg mL-1) was used for the preparation of Tyr-GR-
EMIMAla-Chi/GC enzyme electrode. 5.0 l of the above mixture was cast onto the surface of
freshly polished glassy carbon electrode (GC, 3 mm diameter) to obtain the Tyr-GR-EMIMAla-
Chi/GC electrode. The dried enzyme electrode was stored at 4 °C in a refrigerator when not in
use. Other electrodes were prepared by using similar procedures as described above. A three-
electrode system consisted of the tyrosinase-based GC electrode (3 mm diameter) as the working
electrode, an Ag/AgCl as the reference electrode (KCl concentration: 3 mol L-1), and a platinum
wire as the auxiliary electrode. 50 mmol L-1 phosphate buffer saline (PBS, pH 7.0) was used as
the electrolyte in the electrochemical experiments. Amperometric measurements were carried out
on successive additions of an aliquot volume of catechol solution (1 mmol L-1) into 8 mL stirring
PBS at room temperature (25 °C). The potential applied to the Tyr-GR-EMIMAla-Chi/GC and
Tyr-GO-EMIMAla-Chi/GC working electrode was -0.1 V.
3. Results and Discussion
3.1. Preparation of water-soluble graphene
In our study, a commercially available Graphene (purity~99 ％ ) from Nanjing XFNANO
Materials Tech Co., Ltd (Nanjing, China) was studied. Figure 1(a) shows the TEM image of GR.
Because of the physical preparation method, the obtained GR shows high BET surface area
of >900 m2 g-1 and good electrical conductivity (>1000 s m-1) with a single layer ratio of >80%.
Due to the hydrophobic nature, graphene sheets can’t be dispersed in water and are inclined to
deposit in the bottom, as shown in Figure 1b. The dispersion of graphene in water phase is one
paramount challenge for chemists, which limits its wide application in many fields. Ionic liquids
are compounds consisting entirely of organic cations and inorganic (or organic) anions that exist
in the liquid state around room temperature. As novel attractive solvents, they possess unique
properties such as negligible vapor pressure, wide potential windows, high thermal stability, and
good ionic conductivity and solubility (Buzzeo et al., 2004; Lu et al., 2006). As shown in Table 1,
twelve different kinds of ILs were selected as stabilizer for noncovalent functionalization of GR
sheets through π-π interactions and hydrophobic interaction in water phase. These ILs can be
attributed to imidazolium category or phosphonium category according to their cations, and they
bis(trifluoromethylsulfonyl)amide, or trifluoromethanesulfonate anions. As expected, all the
hydrophobic ILs proved to be not effective on improving the dispersibility of GR in water phase.
On the other hand, the effect of hydrophilic ILs on the dispersibility of GR in water phase is
quite different. For example, 1-ethyl-3-methylimidazolium tetrafluoroborate, which possesses
good hydrophilicity (miscible with water), could improve the dispersion of GR in water phase to
some extent. However, it could not make GR become completely water-soluble. Of the twelve
different ILs, it is interesting to find that AAILs are the most effective ILs that can improve the
dispersion of GR in water. Using amphiphilic 1-ethyl-3-methylimidazolium Alanine (EMIMAla)
or 1-Ethyl-3-methylimidazolium L-Proline (EMIMPro) as stabilizer, stable aqueous dispersions
of GR sheets were obtained since the negatively charged imidazole moiety has strong affinity
with the basal plane of GR viaπ-stacking. Unlike GR (Figure 1b), the AAIL-functionalized GR
became water-soluble and could retain stable in water phase, as shown in Figure 1 (c and d).
After surface functionalization of GR by hydrophilic AAILs, the hydrophobic surface of GR
became hydrophilic. Furthermore, the absorbed imidazolium cations on GR surface result in
strong electrostatic repulsion interaction between GR nanosheets. Previous study revealed that
electrostatic repulsion mechanism played an important role in forming stable GR or GO
dispersions (Li et al., 2008). The formation of stable GR dispersions should be attributed not
only to surface hydrophilicity but also electrostatic repulsion of GR after modification by
charged AAILs. Typically, the dispersion of 0.1 mg ml-1 GR in water will need as much as 10
mg ml-1 sodium dodecylbenzenesulfonate (SDBS) as stabilizer (0.1 mg ml-1 GR vs. 10 mg ml-1
SDBS). In our study, 0.4 mg ml-1 GR can be well dispersed in water phase with the aid of only
3.0 mg ml-1 AAILs (0.1 mg ml-1 GR vs. 0.75 mg ml-1 AAIL). This work, for the first time,
suggests that ordinary graphene, when using AAILs as stabilizer, can be readily dispersed into
water phase to form stable GR dispersion.
3.2. FT-IR characterization of GR, GO and GR-AAIL.
Conventional methods usually improve the dispersion of GR in water by introducing oxygen-
functional group on the surface of GR, which sacrifices the good electronic conductivity of GR.
GR and GO, as shown in Figure 2A. For GO, the characteristic peaks appear at 1055 cm-1 (C-O
stretching peak), 1732 cm-1 (C=O), 1620 cm-1 (the skeletal vibrations of unoxidized graphitic
domains), and 1221 cm-1 (C-OH stretching peak) (Xu et al., 2008; Geng et al., 2010). The FTIR
of GR is quite different from that of GO. As for GR, most of the characteristic peak of oxygen
functional group observed on GO disappear, and a new characteristic peak appears at 1556 cm-1,
corresponding to the C=C bond of the sp2 carbon networks in GR sheet. Figure 2A also shows
the FTIR of GR after modification by AAIL. Almost all the characteristic peaks of EMIMAla
and GR can be found in the GR-EMIMAla nanocomposite, indicating the nanocomposite is
formed by physical interaction instead of chemical covalent function. The band at 1576 cm-1 is
assigned to the characteristic absorption peaks of EMIM[Ala] (i.e., acylamide II). The C-H
vibration for cyclic EMIM+ appears at near 1167 and 623 cm-1. Meanwhile, the relatively
intensive characteristic peaks of EMIMAla at 1405, 843, 3080 cm-1 can also be found in the GR-
EMIMAla nanocomposite, which confirms the presence of EMIMAla in the nanocomposite. The
slight shift of the characteristic peaks of EMIMAla on the nanocomposite indicates the strong
interaction between GR and EMIMAla.
spectra of GR, GR-AAIL and GO clearly displays the structural difference between
3.3. Electrochemical impedance spectroscopy characterization of electronic property
The most significant advantage of the dispersion method in this study is that it does not destroy
the structure integrity of GR, and meanwhile retains the excellent elctronic conductivity of GR.
We carried out EIS measurements to investigate the resistance of the materials towards
heterogeneous charge transfer (Rct). EIS is a very sensitive technique to investigate the ability of
the material to transfer and exchange charges with surrounding molecules (Feng, et al., 2005).
Such electron exchange ability is strongly influenced by the electronic conductivity of the
material. If the electronic conductivity of GR reduced after modification by AAIL, it would be
clearly displayed on the EIS measurement results. Because GR, GO (water-soluble) and GR-
AAIL could not be steadily immobilized on the surface of GC electrode once the modified
electrode was immersed in K3[Fe(CN)6]/K4[Fe(CN)6] electrolyte, Chitosan (Chi) was used as a
film-forming polymer to immobilize the above material on the surface of the GC electrode
steadily. Figure 2B shows the Nyquist diagrams for EIS measurements of GR-Chi, GO-Chi, GR-
EMIMAla-Chi, and Chi modified electrodes in 1 mM K3[Fe(CN)6]/K4[Fe(CN)6] containing 0.5
M KNO3 electrolyte. The charge-transfer resistance (Rct) corresponds to the diameter of the
semicircle in the Nyquist plots obtained from the measurements. As can be seen in Figure 2B,
Chi shows the largest Rct. Compared to Chi, and the Rct of GO-Chi decreases only a little,
indicating the poor electronic conductivity of GO. Because GO contains large amount of oxygen-
containing functional group on the surface, these functional groups destroys its structure integrity
and electronic conductivity. Whereas, the GR-EMIMAla-Chi shows almost a straight line and
the Rct value of GR-EMIMAla-Chi is close to zero, indicating a very small interface electron
resistance. This phenomenon proves that the excellent electronic conductivity of GR-EMIMAla
is preserved. The Nyquist diagram of GR-EMIMAla-Chi is almost the same as that of GR-Chi,
suggesting that the presence of EMIMAla does not make the electronic conductivity of GR
decrease. ILs possess excellent ionic conductivity, which contributes to the good charge transfer
ability of the GR-EMIMAla nanocomposite. GR can interact with EMIMAla via the π-π,
hydrophobic and electrostatic interaction, which results in a stable water-soluble GR with
3.4. Demonstration of Biosensor based on water-soluble GR with high sensitivity
Of great significance is that the successful formation of water-soluble GR enables the use of
conventional solution-phase processing techniques (especially for those biomoleculars
participated process) to create new GR-based materials and devices. These ionic liquids can be
purposely retained or easily removed, depending on different applications. As shown in Figure
3A, the AAIL-functionalized GR was subsequently assembled with tyrosinase biomolecules
(tyrosinase was chosen a model enzyme) for fabricating an electrochemical biosensor. The stable
aqueous dispersion of GR is not only crucial for the assembly process, but also significant for
improving the electrode to electrode reproducibility of different batches. In previous study, GO
was usually used instead of GR for its good dispersion in water phase. In the present study, the
tyrosinase biosensor based on EMIMAla funcctionalized GR ([email protected]
) is compared with
GO-based tyrosinase biosensor for catechol detection. As shown in Figure 3B and 3C, the
detection limit of [email protected]
based biosensor reaches as low as 8 nM with a response time of 3 s.
The detection limit of the developed biosensor is significantly better than that of reported
biosensor based on graphene (750nM, Yin et al., 2011), graphene-Ag nanoparticle (100 nM,
Huang et al., 2013), CNTs (7.6 M, Perez-Lopez and Merkoçi, 2011) and Au nanoparticles (300
nM, Singh et al., 2013). The linear range reaches 3 orders of magnitude from 25 nM to 11100
nM. It should be noted that the sensitivity of [email protected]
based biosensor (12600 mA cm-2 M-1)
is about 17 times higher than that of GO-based biosensor (736 mA cm-2 M-1). Unlike electrically
insulating GO, AAIL-functionalized GR nanosheets retain its intrinsic excellent electronic
conductivity of GR, which can act as electrical nanowires of enzyme electrode to capture the
bioelectrocatalytic signal. The sensitivity of the [email protected]
based biosensor is about 10 times
higher than that of graphene-Ag nanoparticle based nanocomposite (1230 mA cm-2 M-1, Huang
et al., 2013), and 2600 times higher than that of CNTs based biosensor (4.8 mA cm-2 M-1, Perez-
Lopez and Merkoçi, 2011). The sensitivity of the developed biosensor is also much higher than
that of biosensor based on graphene (7634 mA cm-2 M-1, Qu et al., 2013), mesocarbon (1385 mA
cm-2 M-1, Wu et al., 2012) and mesocarbon-Co3O4 nanocomposite (6400 mA cm-2 M-1, Wang et
al., 2014). Compared to conventional GR, GO, CNTs and other nanomaterials, the advantages of
AAIL-functionalized GR are significant. Amino acid ionic liquid functionalized graphene proves
to be a robust electrochemical biosensing platform for ultrasensitive biosensing applications.
3.5. Reproducibility, Selectivity, Stability and real sample application of the biosensor
The repeatability of the biosensor was investigated by amperometry. The relative standard
deviation (R.S.D.) of the biosensor response to 300 nM catechol for 7 successive measurements
was 2.6%, indicating good repeatbility. To evaluate the electrode-to-electrode reproducibility,
three biosensors were prepared under the same conditions independently. The R.S.D. of the
prepared biosensors was 3.5%, indicating good electrode-to-electrode reproducibility. The good
water phase dispersion of AAIL-functionalized graphene contributes to the good electrode-to-
electrode reproducibility. The influence of matrix on the biosensor response was also evaluated
in the PBS (pH 7.0) containing 0.3 M catechol in the presence of 3M interferents. It was
found that ethanol, glucose, sucrose, ascorbic acid, uric acid and inorganic ions (K+, Na+, Ca2+,
NO3-, PO4-, Cl — , Ac-, etc.) did not cause any interference. The good selectivity should be
ascribed to the intrinsic selectivity of tyrosinase for catechol substrate and the applied low
potential (-0.1V). The long-term stability of the biosensor was investigated over a 35-day period.
When the biosensor was stored dry at 4 oC and measured intermittently (twice every week), the
current response to 300 nM catechol decreased about 5% over a 35-day period. AAILs are
biocompatible ionic liquids (Wu et al., 2012). The good long-term stability can be attributed to
the excellent biocompatibility of the nanocomposite, which can provide a favorable
microenvironment for tyrosinase to retain its bioactivity. Both biocompatibility and inherent
conductivity of the nanocomposite enable it to become an excellent biosensing platform for
enzymes along with good stability.
The biosensor was further used to detect real environmental water samples. The recovery test
was studied by adding spiked catechol into tap water and river water. River water samples were
collected from Daliao River (Liaoning). Water samples were transported to the laboratory and
were stored at 4 oC in glass containers before analysis. Tap water samples were taken from our
laboratory (Dalian). All samples were filtered through 0.45 μm filter membrane before use in
order to remove suspended solids. When the concentrations of catechol were from 300 nM to
10000 nM, the recovery was from 90.5% to 108.6% and the RSD was from 2.2% to 6.0 % for tap
water and river water. The results confirm that the fabricated biosensor is applicable for real
In summary, a simple method was developed for preparing water-soluble graphene by using
amphiphilic ILs for the non-covalent surface modification of graphene through π-π interactions.
After physical modification by AAILs, the hydrophobic GR became water-soluble and displayed
long-term stability in water-phase without deposition. Unlike conventional method, the greatest
advantage of the present method is that it can retain the excellent electronic conductivity and
structure integrity of GR. Our findings make it possible to process graphene materials using low-
cost solution processing techniques, opening up enormous opportunities to use this unique
carbon nanostructure for many technological applications. The obtained water-soluble GR was
exemplified to fabricate an electrochemical tyrosinase biosensor, and displayed its superior
advantage to GR, GO and CNTs based biosensor with higher sensitivity and better detection
limit. The AAIL-GR based biosensor also demonstrated good reproducibility, selectivity and
long-term stability for catechol detection. The recovery for real water samples was from 90.5%
to 108.6%, confirmed that the biosensor was applicable for real samples detection. The GR-
AAIL nanocomposite provides a versatile and robust platform for fabricating ultrasensitive
biosensors with excellent performance. The discovery in this study might inspire wide
application of graphene in many fields, such as nanoelectronics, sensors, biosensors,
supercapacitors, and catalysis.
This work was supported by the National Natural Science Foundation of China (No 20907051),
the National High Technology Research and Development Program of China (2013AA065203),
and the Knowledge Innovation Program of the Chinese Academy of Sciences (No DICP
Baughman, R. H., Zakhidov, A. A., de Heer, W. A., 2002. Science 297, 787.
Buzzeo, M. C., Hardacre, C., Compton, R. G., 2004. Anal. Chem. 76, 4583.
Feng, J. J., Zhao, G., Xu, J. J., Chen, H. Y. 2005. Anal. Biochem. 342, 280.
Geng, J., Liu, L., Yang, S. B., Youn, S.C., Kim, D. W., Lee, J.S., Choi, J.K., Jung H.T., 2010. J.
Phys. Chem. C 114, 14433.
Gholivandn, M. B., Khodadadian, M., 2014. Biosen. Bioelectron. 53, 472.
Huang, K., Wang, L., Li , J., Yu, M., Liu, Y.M., 2013. Microchim Acta. 180, 751.
Li, D., Muller, M.B., Gilje, S., Kaner R.B., Wallace G. G., 2008. Nature Nanotechnology 3, 101.
Liu, F., Piao, Y., Choi, J.S., Seo, T.S. 2013a. Biosen. Bioelectron. 50, 387.
Liu, N., Chen, X., Ma, Z., 2013b. Biosen. Bioelectron. 48, 33.
Lotya, M., Hernandez, Y., King, P. J., Smith, R. J., Nicolosi, V., Karlsson, L. S., Blighe, F. M.,
De, S., Wang, Z., McGovern, I. T., Duesberg, G. S., Coleman, J. N., 2009. J. Am. Chem.
Soc. 131, 3611.
Lou, W.Y., Zong, M.H., Wu, H., 2004. Biocatal. Biotransform. 22 171.
Lu, X., Hu, J., Yao, X., Wang, Z., Li. J., 2006. Biomacromolecules 7, 975.
Lu, X.B., Zhang, Q., Zhang, L., Li. J.H., Electrochem. Commun., 2006, 8, 874.
Malig, J., Romero-Nieto, C., Jux, N., Guldi, D. M., 2012. Adv. Mater. 24, 800.
Moulthrop, J. S., Swatloski, R. P., Moyna, G., Rogers, R. D. 2005. Chem. Commun., 1557
Park, S., Ruoff, R. S., 2009. Nature Nanotechnology 4, 217.
Perez-Lopez, B., Merkoçi, A., 2011. Adv. Funct. Mater. 21, 255
Ponomarenko, L. A., Schedin, F., Katsnelson, M. I., Yang, R., Hill, E. W., Novoselov, K. S.,
Geim, A. K., 2008. Science 320, 356.
Qu, Y., Ma, M., Wang, Z., Zhan, G., Li, B., Wang, X., Fang, H., Zhang, H., Li, C., 2013. Biosen. Bioelectro. 44, 85.
Si, Y., Samulski, E. T., 2008. Nano Lett. 8, 1679.
Singh, S., Jain, D. V. S., Singla, M. L., 2013. Sens. Actuators B, 182, 161.
Sun, Y. P., Fu, K. F., Lin, Y., Huang, W., 2002. J. Acc. Chem. Res. 35, 1096.
Wang, X., Lu, X., Wu, L., Chen, J., 2014. ChemElectroChem, 1, 808.
Wu, L.D., Deng, D., Jin, J., Lu, X.B., Chen, J.P., 2012b. Biosen. Bioelectron. 35, 193.
Wu, L., Lu, X., Zhang, H., Chen, J., 2012a. ChemSusChem. 5, 1918.
Xu, Y., Bai, H., Lu, G., Li, C., Shi, G., 2008. J. Am. Chem. Soc. 130, 5856.
Yin, H.S., Zhang, Q.M., Zhou, Y.L., Ma, Q., Liu, T., Zhu, L.S., Ai, S.Y., 2011. Electrochim
Acta 56, 2748. Zhou, Q., Yang L., Wang, G., Yang, Y., 2013. Biosen. Bioelectron. 49, 25.
Figure and Table Captions.
Table 1. Twelve different kinds of ILs selected for investigation.
Figure 1. TEM image of graphene (a) and images of water dispersions (0.4 mg mL-1) of
graphene (b), EMIMPro functionalized graphene (c), and EMIMAla functionalized graphene (d).
IL concentraton: 3.0 mg/ml.
Figure 2. (A) FT-IR
(GR-EMIMAla); (B) Nyquist diagrams for EIS measurements of GR-Chi, GO-Chi, GR-
EMIMAla-Chi, and Chi modified electrodes. Conditions: 1 mM K3[Fe(CN)6]/K4[Fe(CN)6]
containing 0.5 M KNO3 supporting electrolyte. Inset: Randles equivalent circuit used for data
Figure 3. (A) Schematic diagram for the preparation of AAIL-functionalized graphene and
subcequent assembly with tyrosinase biomolecules; (B) The typical amperometric response and
(C) the calibration curve of the tyrosinase biosensors based on EMIMAla-functionzalized
graphene ([email protected]
) and GO for catechol detection.
spectra of pristine GR, GO, EMIMAla, and EMIMAla functionalized GR
Table 1. Twelve different kinds of ILs selected for investigation ILs
Trihexyl(tetradecyl) phosphonium tetrafluoroborate
360 361 362 363 364
1405 1167 1576
1620 1732 1221 1055
-1 Wavenumber (cm )
372 373 374 375
376 377 378 379
(A) [email protected]
GO [email protected]
6 4 2 0
6 4 2 0
380 381 382
400 600 Time (s)
383 384 385 386
Figure. 3. Highlights
A non-covalent method was developed for preparing water-soluble graphene.
Results confirmed the water-soluble graphene retained excellent electronic conductivity.
The graphene dispersions enable the use of conventional solution-phase processing
391 392 393 394
techniques. A robust biosensing platform was developed based on amino acid ionic liquid functionalized graphene. The biosensing platform displayed excellent performance for biosensor application.